Int. J. Electrochem. Sci., 7 (2012) 7976 - 7983
International Journal of
A Comparative Study of Nanoparticles and Nanospheres
as Anode Material for Lithium Ion Batteries
Huayun Xu, Xianglan Chen, Liang Chen, Li’e Li, Liqiang Xu, Jian Yang*
, Yitai Qian
Shandong Univ, Key Lab Colloid & Interface Chem, Minist Educ, Sch Chem & Chem Engn, Jinan 250100, Peoples R China
Received: 9 July 2012 / Accepted: 30 July 2012 / Published: 1 September 2012
Spinel structure ZnFe2O4 were prepared by hydrothermal and solvothermal methods. Investigations on
X-ray diffraction (XRD) and transmission electron microscopy (TEM) indicate that the samples are well-crystallized cubic ZnFe2O4 with average nanoparticle size ranging from 30 to 90 nm and
nanosphere size in the range of 200~250 nm composed of around 20 nm nanoparticles with increasing sintered temperature for hydrothermal and solvothermal method, respectively. The ZnFe2O4 samples
sintered at 600 oC show high lithium-storage capacity and good reversibility. Compared with nanoparticles, ZnFe2O4 nanospheres demonstrate a reversible capacity over 860 mAh g-1 and good rate
capability. Electrochemical impedance spectroscopy (EIS) was carried out and decreased warburg impedance was found for nanospheres compared to nanoparticle ZnFe2O4.
Keywords: ZnFe2O4; Nanostructured materials; Lithium ion battery; Electrochemical impedance
Transition metal oxides such as Fe3O4 [6, 7] and ferrites with general formula AFe2O4 (A: Zn,
Ni, Co, Cu, Cd) [8–16] have been widely investigated as promising anode materials for high-power lithium-ion batteries due to their relatively high theoretical capacities (600~1000 mAh g-1). Among them, ZnFe2O4 shows a high reversible capacity (theoretical capacity: 1072 mAh g-1, according to 9
moles Li per mole of ZnFe2O4) because Zn can contribute additional capacity due to
alloying-de-alloying reaction besides buffering the volume variation during conversion reaction [12, 13, 17, 18]. But itsuffers from structure instability owing to volume change during charge /discharge course, low electron conductivity and aggregation of the particles caused by charge/discharge cycles . As we know, nanoscale structure can effectively shorten Li+ insertion/extraction pathways and morphology of electrode material plays an important role on the electrochemical performance for Li-ion batteries [12, 19-21]. Chen synthesized hollow sphere ~1μm in diameter shows reversible capacity 900 mAh . Nuli reported nanofilm ZnFe2O4 by laser deposit method retaining reversible capacity of 432 mAh g-1 g
after 100 cycles . Chowdari found cubic ZnFe2O4 with a particle size range of 100~300 nm
obtained by urea combustion performs 615 mAh g-1 after 50 cycles .
In our work, we synthesized cubic ZnFe2O4 by hydrothermal and solvothermal method and
investigated the structure and morphology by XRD and TEM. Electrochemical performance tests and EIS were carried out and improved cycling capability and decreased warburg impedance were found for nanospheres ZnFe2O4 compared to nanoparticles ZnFe2O4.
2. EXPERIMENTAL 2.1 Synthesis
All reagents were analytical grade and used without further purification. 2 mmol FeCl3·6H2O
and 1 mmol ZnCl2 were mixed under vigorously stirring and adjusted pH by NaOH solution to 9. Then
transferred to a Teflon-lined stainless steel autoclave (60 mL) and heated at 200 oC for 24 h. The product was collected by centrifugation, washed with distilled water and ethanol, and dried at 80 oC in air for 8 h. Finally the powders were annealed at 500 oC, 600 oC and 700 oC for 3 h. For solvothermal method, the difference is using ethyl alcohol as solvent and adding 10 mmol urea into the FeCl3·6H2O
and ZnCl2 solution instead of controlling pH using NaOH solution.
XRD patterns of the samples were provided using a Bruker D8 advanced X-ray diffractometer with Cu Kα radiation (λ=1.5418 Ǻ). The ZnFe2O4 samples were observed on a transmission electron
microscope (TEM, JEOL-2010). The coin cells comprised of the prepared powder as cathode, lithium as anode, and an electrolyte having 1M LiPF6 in an ethylene carbonate (EC)-diethyl carbonate
Zahner Elektrik IM6 (Germany) impedance instrument over the frequency range of 100 kHz to 0.01Hz.
3. RESULTS AND DISCUSSION
Figure 1. XRD patterns of the ZnFe2O4 as prepared samples and then sintered at different temperature
samples synthesized by hydrothermal (A) and solvothermal method (B)
Figure 2. TEM of the ZnFe2O4 as prepared samples (a) and then sintered at different temperature
XRD analysis (Figure 1A and 1B) indicates that the powders by two routes sintered at 500~700
C is phase-pure cubic ZnFe2O4 (JCPDS card No. 65-3111). It is obvious that with increasing the
calcination temperature, the peak becomes sharp which means strengthened crystallization.
Figure 2 shows the TEM of the ZnFe2O4 as prepared and then sintered at different temperature
samples synthesized by hydrothermal (Figure 2A) and solvothermal method (Figure 2B). As shown in Figure 2A, the powder obtained from hydrothermal method are composed by agglomerated nanoparticles with average size ranging from 30 nm to 90 nm around with the increasing sintered temperature. Similar morphology was also reported by polymer pyrolysis method and sol–gel auto-combustion method [21, 22]. TEM imaging (Figure 2B) demonstrates that the powder synthesized by solvothermal method are composed of well-dispersed spheres around 200 nm in diameter and the size of its primary particles is changed from less than 10 nm to around 20 nm. On the other hand, based on Scherrer formula, we calculated the grain size of ZnFe2O4 to be 24 nm around for powder obtained
from solvothermal route, which is consistent with TEM result. It is also can be seen that with increased sintering temperature, the very thin nanofibers and small nanoparticles gradually disappears and becomes the ingredients of nanophere.
Figure 3. The first charge-discharge curve for as prepared ZnFe2O4 and then sintered at different
temperature samples synthesized by hydrothermal (A) and solvothermal method (B)
Figure 3 shows the initial charge and discharge profile for as prepared ZnFe2O4 and then
sintered at different temperature samples synthesized by hydrothermal (Figure 3A) and solvothermal method (Figure 3B) tested at 50 mA g-1 between 0.005-3.0V. It is clear that the initial discharge capacity for all ZnFe2O4 samples is around 1200 mAh g-1. It is high than 1072 mAh g-1 according to 9
lithium insertion, which might be attributed to the nature of the material and the formation of a solid electrolyte interphase (SEI) on the electrode surface due to the decomposition of the electrolyte .
Figure 4 shows the discharge capacity as a function of cycle for as prepared ZnFe2O4 and then
Figure 4. Discharge capacity as a function of cycle for as prepared ZnFe2O4 and hen sintered at
different temperature samples synthesized by hydrothermal (A) and solvothermal method (B)
Figure 5. The discharge capacity as a function of cycle for 600 oC sample obtained by different method
The tested current is 50 mA g-1 and cut-off voltage is between 0.005-3.0V. Sample sintered at 600 oC obtained respectively from two different routes show the highest capacity and the best cycle performance. Comparing the cycle performance for 600 oC sintered sample obtained by two different methods as shown in Figure 5, it is obvious that the capacity maintaining for nanospheres is much better than that of nanoparticles. After 50 cycles, the capacity of nanospheres is over 500 mAh g-1, while only around 300 mAh g-1 was maintained for nanoparticles ZnFe2O4. Though the capacity
that nanospheres composed by small nanoparticles are contributed to the structure stability by impress the volume changes during charge and discharge course.
Figure 6. Rate capacity of 600 oC samples obtained by different methods between 0.005 and 3.0 V at various current densities
Figure 6 shows the rate capacity of 600 oC samples obtained by different method between 0.005 and 3.0 V at various current densities. ZnFe2O4 nanospheres perform higher capacity at various
current densities from 50 mA g-1 to 600 mA g-1 compared to nanoparticles. Moreover, when the current density decreases to 50 mA g-1 again, nanospheres show more reversible than nanoparticles do, which is believed that ZnFe2O4 nanospheres composed of small nanoparticles (Figure 2B) are
contributed to the structure maintaining during conversion reaction.
Table 1. Rs, Rct and Zw value of the ZnFe2O4 nanoparticles and nanospheres
EIS was performed to investigate the electrode resistance information for 600 oC sintered samples obtained by two different methods as presented in Figure 7a. The equivalent circuit for modeling impedance data is shown in Figure 7b. The intercept at the real (Z’) axis in high frequency corresponds to the ohmic resistance (Re). The semicircle in the middle frequency range indicates the
charge transfer resistance (Rct) and the inclined straight line relates to the Warburg impedance (Zw).
The fitting results are presented in Table 1. The Rct value of the ZnFe2O4 nanoparticles and
nanospheres is 249.7Ω and 234.5 Ω, respectively. The Zw value for nanoparticles is 233.4 Ω, while
only 155.2 Ω for nanospheres. Clearly, the nanospheres ZnFe2O4 can suppress the warburg impedance
which related to lithium ion diffusion in the solid state electrode material. Decreased warburg impedance means faster lithium ion diffusion for nanospheres compared to nanoparticle and then contributed to a higher discharge capacity and rate capability compared to the nanoparticles ZnFe2O4
(shown in Figure 5 and 6).
In summary, hydrothermal and solvethermal methods have been developed to prepare ZnFe2O4
spinel material. Comparing the structure, morphology and electrochemical performance, it is found that nanospheres via solvethermal route performs higher specific capacity, improved cyclability and good rate capability compared to nanoparticles obtained from hydrothermal method. It is believed that the morphology of nanopheres composed of small nanoparticles is contributed to good electrochemical performance for ZnFe2O4 anode material. ZnFe2O4 nanospheresshow high first discharge and charge
anode material in LIBs, and further improvement by carbon materials such as graphene for nanopheres ZnFe2O4 is under investigation in our work.
This study was supported by the 973 Project of China (No.2011CB935901), the National Natural Science Foundation of China (Grant No. 11179043, No. 91022033), the Independent Innovation Foundations of Shandong University (2011GN032, 2012ZD007), Shandong Provincial Natural Science Foundation for Distinguished Young Scholar and start-up funding for new faculties in Shandong University. We are also grateful to the Graduate Independent Innovation Foundation of Shandong University (yzc11034).
1. S.L. Yang, H.H. Song, X.H. Chen, J. Power Sources 173 (2007) 487-494.
2. Y.S. Wu, Y.H. Wang, Y.H. Lee, J. Alloy. Compd. 426 (2006) 218-222. 3. D. Guerard, R.. Janot, J.Ghanbaja, P. Delcroix, J. Alloy. Compd. 434 (2007) 410-414. 4. M.S. Sh, F. Golestani, H.Sarpoolaky, J. Alloy. Compd. 482 (2009) 361-365.
5. M.A.Worsley,S.O.Kucheyev,J.H.Satcher,A.V.Hamza,T.F. Baumann, Appl. Phys. Lett. 94 (2009) 73-77.
6. L. Taberna, S. Mitra, P. Poizot, P. Simon, J.M. Tarascon Nat. Mater. 5 (2006) 567-573. 7. S.B. Ni, D.Y. He, X.L. Yang, J. Alloy. Compd. 509 (2011) L305-L307.
8. R. Alcántara, M. Jaraba, P. Lavela, J. L. Tirado, J. C. Jumas, J. Olivier-Fourcade, Electrochem. Commun. 5 (2003) 16-21.
9. Y. Q. Chu, Z. W. Fu, Q. Z. Qin, Electrochim. Acta 49 (2004) 4915-4921.
10. M. Bomio, P. Lavela, J. L. Tirado, J. Solid State Electrochem. 12 (2008) 726-731. 11. C. Q. Hu, Z. H. Gao, X. R. Yang, J. Magn. Magn. Mater. 320 (2008) L70-L73.
12. X. Guo, X. Lu, X. Fang, Y. Mao, Z. Wang, L. Chen, X. Xu, H. Yang, Electrochem. Commun. 12 (2010) 847-850.
13. Y. Sharma, N. Sharma, G.V. Subba Rao, B.V.R. Chowdari, Electrochim. Acta 53 (2008) 2380-2385.
14. P. Lavela, J.L. Tirado, J. Power Sources 172 (2007) 379-387.
15. R. Kalai Selvan, N. Kalaiselvi, C.O. Augustin, C.H. Doh, C. Sanjeeviraja J. Power Sources 157 (2006) 522-527.
16. Y. Sharma, N. Sharma, G.V. Subba Rao, B.V.R. Chowdari Bull Mater Sci 32 (2009) 295-304. 17. Y. Sharma, N. Sharma, G.V. Subba Rao, B.V.R. Chowdari, Adv. Funct. Mater. 17 (2007)
18. Y. Yang, Y Zhao, L. Xiao, L. Zhang Electrochem. Commun. 10 (2008) 1117-1120. 19. Y. N. NuLi, Y. Q. Chu, Q. Z. Qin, J. Electrochem. Soc. 151 (2004) A1077-A1083.
20. L. M. Jin, Y. C. Qin, H. Deng, W. S. Li, H. Li, S. H. Yang, Electrochim. Acta 56 (2011) 9127-9132.
21. C.T. Cherian, M. V. Reddy, G. V. S. Rao C.H. Sow, B.V.R. Chowdari, J. Solid State Electrochem 16 (2012) 1823-1832.
22. Y. Ding, Y.F. Yang, H.X.Shao, Electrochim. Acta 56 (2011) 9433-9438.
23. Y. F. Deng, Q. M. Zhang, S. D. Tang, L. T. Zhang, S. N. Deng, Z. C. Shi, G. H. Chen, Chem. Commun. 47 (2011) 6828-6830.